J. Phys. Chem. C 2009, 113, 17156–17159
Structural and Electronic Properties of Au Induced Nanowires on Ge(001) Daan Kockmann, Tijs F. Mocking, Arie van Houselt, Bene Poelsema, and Harold J. W. Zandvliet* Physical Aspects of Nanoelectronics and Solid State Physics, MESA+ Institute for Nanotechnology, P. O. Box 217, 7500 AE Enschede, The Netherlands ReceiVed: July 10, 2009; ReVised Manuscript ReceiVed: August 21, 2009
The structural and electronic properties of Au induced self-organized nanowires on Ge(001), prepared by different procedures, are investigated with scanning tunnelling microscopy and spectroscopy at room temperature and 77 K. We find that the Au induced nanostructures are identical for the different preparation procedures. The Au induced nanowires are comprised of dimers that have their bond aligned in a direction perpendicular to the nanowire. The dimers are buckled, leading to a 2× periodicity along the nanowires. Dimers located at antiphase boundaries are dynamic and flip back and forth between two buckled configurations. The troughs between the nanowires have a depth of several atomic layers. Finally, the differential conductivities of the nanowires and the troughs are very comparable in magnitude. Introduction The properties of electron systems become increasingly exotic as one progresses from the three-dimensional (3D) case into lower dimensions. In 2D electron systems novel and intriguing physical phenomena, such as the integer1 and fractional quantum Hall effect,2,3 have been found. More recently, the realization of a single layer of graphite (graphene) has resulted in a wealth of unexpected and exciting physical phenomena.4 For instance the electron transport in graphene is governed by the relativistic Dirac equation rather than by the Schro¨dinger equation.5 The predictions for 1D electron gases lead to even more exotic properties. The Fermi liquid approach breaks down spectacularly in one dimension.6,7 It has been predicted that the 1D electron gas is much better described by the Luttinger liquid formalism. One of the intriguing predictions of a Luttinger liquid is that the electron loses its identity and separates into two collective excitations of the quantum mechanical many body systems: a spinon that carries spin without charge, and a holon that carries the positive charge of a hole without its spin. The major problem with 1D electron systems is that they are much harder to realize than their 2D and 3D counterparts. The ideal 1D system would be a freely suspended atomic chain. Using the quantum mechanical break junction approach such freely suspended atomic chains can indeed be made.8 However, the maximum length of these atomic chains is limited to only a few atoms. As an alternative, atomic chains can be created on surfaces either via self-organization,9,10 step decoration,11 or atom-by-atom manipulation12 using scanning tunnelling microscopy (STM). In order to electronically decouple the electrons near the Fermi level from the underlying substrate often a material with a band gap is chosen.13-15 Examples that fall in this category are Pt and Au induced one-dimensional structures on Ge(001) surfaces.16-20 Wang and co-workers17,18 reported the formation of a zigzag Au dimer row upon deposition of Au on Ge(001). Recently, Scha¨fer and co-workers19 reported that the deposition of Au on Ge(001) leads to the formation of Au chains with a diameter of * To whom correspondence [email protected]
only a single atom, which represent an outstandingly close approach to a one-dimensional electron liquid. These authors report a change of the tunnelling conductivity by 2 orders of magnitude when comparing the ridges of the self-organized nanowires with the troughs in between the nanowires. Their preparation method is, however, somewhat different from the one used by Wang et al.17,18 and van Houselt et al.20 Since there is some controversy regarding the exact structural and electronic properties of the Au induced nanowires prepared by the different research groups we have revisited this system by comparing the Au induced nanowires that have been prepared by the different preparation procedures. In this article, we compare two preparation procedures, namely (1) deposition of Au at 775 K and (2) deposition of Au at room temperature followed by an anneal at 650 K. The first method is applied by Schafer et al.,18 whereas Wang et al.17,18 and van Houselt et al.20 used the second method. On the basis of STM and scanning tunnelling spectroscopy (STS) measurements, we found that the resulting structures are in both cases electronically and structurally identical. In agreement with both Wang et al.17,18 and Scha¨fer et al.19 the Au induced nanowires are 1.6 nm separated apart. However, the height of these structures turns out to be at least 5 Å, i.e., several atomic layers, rather than the one layer (1.5 Å) reported by Scha¨fer et al.19 and Wang et al.17 Furthermore, in agreement with Wang et al. we found that the Au induced nanowires are two atoms wide rather than one atom. Finally, our experiments reveal that the differential conductivities of the nanowires and the regions in between the nanowires are very comparable in magnitude. Experimental Section Experiments were performed with a low-temperature and a room-temperature STM from Omicrometer (LT-STM and STM1) both operating in ultrahigh vacuum (UHV). Ge(001) substrates were cut from nominally at 3 in. by 0.5 mm, about 25 Ω · cm resistance, single-side-polished n-type wafers. Samples were mounted on Mo holders and contact of the samples to any other metal during preparation and experiment has been carefully avoided. The Ge(001) samples were cleaned by prolonged 800 eV Ar+ ion sputtering and annealing via resistive
10.1021/jp906536a CCC: $40.75 2009 American Chemical Society Published on Web 09/10/2009
Structural and Electronic Properties of Au Induced Nanowires on Ge(001)
Figure 1. STM image of an array of Au induced nanowires on a Ge(001) surface taken at room temperature. The Au induced nanowires are prepared by deposition of Au on the Ge(001) surface at 775 K. The ellipses mark dimers that exhibit a flip-flop motion during imaging. Sample bias is -0.5 V, tunnelling current is 0.4 nA, and the image size is 12.5 nm × 12.5 nm. Inset: Line scan taken along the indicated arrow. The depth of the troughs is about 0.4-0.5 nm and thus involves several atomic layers.
heating at 1100 ((25) K. The temperature was measured with a pyrometer. After several cleaning cycles the Ge(001) samples were atomically clean and exhibited a well ordered (2 × 1)/c(4 × 2) domain pattern.21,22 We have applied two methods to prepare the Au induced self-organizing one-dimensional structures. In the first method an equivalent of ∼0.5 monolayers of Au was deposited onto the surface at 775 ((25) K. Au was evaporated by resistively heating a W wire wrapped with highpurity Au (99.995%). In the second method an equivalent of ∼0.5 monolayers of Au was deposited at room temperature. After Au deposition the sample was annealed at 650 ((25) K for 2 min and then cooled down to room temperature by radiation quenching before placing it into the STM for observation. Results and Discussion In Figure 1 an STM image of an array of Au induced nanowires on a Ge(001) surface is depicted. An equivalent of ∼0.5 monolayers of Au was deposited on a Ge(001) sample kept at a temperature of 775 K. After being cooled down to room temperature, the sample was imaged with STM. The Au induced nanowires appear as bright zigzag rows in the image. Occasionally defects in the rows are observed. One also finds occasionally noisy appearing dimers in the rows (marked by ellipses). A line profile recorded in a direction perpendicular to the nanowire direction is shown in the inset of Figure 1. The depth of the troughs is about 0.4-0.5 nm and thus involves several atomic layers. It should be pointed out here that one needs a very sharp STM tip in order to measure the depth of the troughs between the densely packed nanowires. With a blunt tip the extracted trough depth will of course be significantly smaller. Subsequently we deposited ∼0.5 monolayer of Au on a fresh Ge(001) sample kept at room temperature. After the deposition process the sample was annealed at 650 K for 2 min. In Figure 2 an STM image of the Au induced nanowires is depicted. The image has the same characteristics as mentioned for Figure 1: The Au induced nanowires appear as bright zigzag rows in the
J. Phys. Chem. C, Vol. 113, No. 39, 2009 17157
Figure 2. STM image of an array of Au induced nanowires on a Ge(001) surface taken at room temperature. The Au induced nanowires are prepared by deposition of Au at room temperature followed by annealing at 650 K. The ellipses mark dimers that exhibit a flip-flop motion during imaging. Sample bias is -1.0 V, tunnelling current is 0.6 nA and the image size is 12.5 nm × 12.5 nm. Inset: Line scan taken across the indicated arrow. The depth of the troughs is about 0.4-0.5 nm and thus involves several atomic layers. The monatomic step height on Ge(001), δ () 0.14 nm), is also indicated.
image, occasionally interrupted by defects and noisy appearing dimers (marked by ellipses). A line scan taken in a direction perpendicular to the nanowires is shown in the inset of Figure 2. The height is calibrated at a monatomic step of the bare Ge(001) surface, which has a height of 0.14 nm. Again the depth of the troughs is about 0.4-0.5 nm and thus involves several atomic layers. The deposition of ∼0.3 monolayer Au leads for both preparation procedures to a surface containing nanowire and nanowire-free regions, whereas the deposition of more than a 1-1.5 monolayer of Au results in the coexistence of nanowire regions and rectangular-shaped 3D clusters.18 For growth or anneal temperatures that exceed 1000 K no nanowires are found. First, we discuss the structure of Au induced nanowires. In ref 20 van Houselt and co-workers proposed a model for the Au induced nanowires, prepared by annealing at 650 K after Au deposition at room temperature (see for Figure 2), where the ridges of the nanowires consist of Ge dimers and the troughs are Au decorated Ge(111) facets. The STM images shown in Figures 1 and 2 are very comparable and thus provide strong evidence for the fact that the structure of the Au induced nanowires is independent of the preparation method. The idea that the Au induced nanowires are comprised of buckled dimers, leading to a 2× periodicity along the nanowire direction, has already been put forward in the first paper on the Au/Ge(001) system by Wang et al.17 In Figures 1 and 2 zigzag lines that refer to the buckling registry in the Au induced nanowires are shown. Occasionally antiphase boundaries in the buckling registry are observed, leading to a single dimer that flips back and forth between the two buckled states, since this dimer does not know whether to align with its left or right neighbor. These flip-flopping dimers have a frizzy appearance and are present in Figures 1b and 4 of ref 20, as well as Figures 1 and 2 of the current work (they are marked by ellipses). Moreover, they are also observable in Figure 2a of ref 17. A detailed analysis of
J. Phys. Chem. C, Vol. 113, No. 39, 2009
Kockmann et al.
Figure 3. STM images of Pt induced (a) and Au induced (c) nanowires and of a pristine Ge(001) surface (e). The images are 5 nm × 5 nm, sample biases are -1.0 V for (a) and (c) and -1.5 V for (e). Tunneling currents are 0.4 nA for (a) and (e) and 0.6 nA for (c). Line scans along the indicated arrows are shown in (b), (d), and (f).
the distribution of the residence times in the two buckled states reveals20 that the flip-flop process is a stochastic process. The Ge dimers of the pristine Ge(001) surface are also known to exhibit such a stochastic flip-flop motion.23 The buckling of the dimers leads to a periodicity of 0.8 nm along the nanowires. Scha¨fer et al.19 observed the same periodicity along the nanowire direction. However, on the basis of an analysis of the Full Width at Half-Maximum (FWHM) of the Au induced nanowires, which was measured to be 0.72 ( 0.03 nm, they concluded that the nanowires have a width of only one atom. In Figure 3 STM images of the Pt induced, see refs 9, 16, and 24, (a) and Au induced nanowires (b) and of the pristine Ge(001) surface (c) are shown for comparison. The spacing between neighboring Pt and Au nanowires is in both cases 1.6 nm. The FWHM differs substantially, from only 0.45 nm for the single atom wide Pt nanowires (Figure 3b) to 0.75 nm for the Au induced nanowires (Figure 3d). The latter value is very similar to the FWHM of the Ge dimers of the pristine Ge(001) surface (Figure 3f). On the basis of the data shown above, we arrive at the conclusion that the Au induced nanowires are not one atom wide, but two atoms (i.e., a dimer). In addition, in Figure 3b an additional atomic structure within the troughs is visible, located at the side of the nanowires. These small blobs are, in most cases, 2.4 nm separated apart and alternately located at left and right sides of the trough. As detailed in ref 20, we suggested that these structures arise at the antiphase-boundaries in the Au covered Ge(111) facets. As can be concluded from the STM data presented in Figures 1 and 2 the structural properties of the Au induced structures for both growth methods are identical. The STM images of the Au induced structures in refs 17-20 show nevertheless some variation in appearance. How to account for these differences? From Figures 1 and 2 it is evident that the Au induced nanowires can actually be considered as a comb of sharp ridges. The obtained STM images of such a surface will certainly be convoluted with the shape of the STM tip. The latter will lead to variety of STM images, since the exact tip shape is in general not known and can not be precisely controlled. By taking many STM images with different STM tips on a Ge(001) surfaces with Au induced nanowires we have been able to reproduce figures which closely resemble the images shown in Figure 2a of ref 17 (see Figure 4a) and Figure 1b of ref 19. These findings support the idea that the structural properties of the Au induced
Figure 4. STM images of Au induced nanowires prepared by Au deposition at 775 K. The image in (a) resembles Figure 2a of ref 17. Image size is 10 × 10 nm, sample bias -0.9 V, tunneling current 3.0 nA. The image in (b) resembles Figure 1b of ref 19. Image size is 15 × 15 nm, sample bias 0.7 V, tunneling current 0.4 nA.
nanowires prepared by the two different perperation methods are indeed similar. Next, we focus on the electronic properties of the Au induced structures. In ref 20 we have pointed out that the local density of states of the Au induced nanowires resembles the local density of states of the bare Ge(001) surface very well,25 suggesting that the Au induced chains are comprised of pure Ge dimers
Figure 5. dI/dV curves recorded on top of the Au induced nanowires and in the troughs between the Au induced nanowires at 77 K (set point voltage is -1.8 V and set point current is 0.5 nA) and at room temperature (set point voltage is -1.5 V and set point current is 0.7 nA).
Structural and Electronic Properties of Au Induced Nanowires on Ge(001) rather than pure Au or mixed Au-Ge dimers. In Figure 5 the differential conductivities, dI/dV, recorded at 300 and 77 K on top and in between the Au induced nanowires are shown. The differential conductivities at the Fermi edge on the nanowires and in the troughs are very comparable in magnitude. In order to compare the differential conductivities at various locations on the surface properly it is important to record the IV traces at a fixed sample bias and tunnel current setpoint. Interestingly, Scha¨fer et al.19 reported a difference of not less than 2 orders of magnitude in the differential conductivities of the nanowires and the troughs. We are only able to reproduce these results if we use different values for the setpoint values.
J. Phys. Chem. C, Vol. 113, No. 39, 2009 17159
References and Notes
(2) Tsui, C.; Stormer, H. L.; Gossard, A. C. Phys. ReV. Lett. 1982, 48, 1559. (3) Langlin, R. B. Phys. ReV. Lett. 1983, 50, 1395. (4) Geim, A. K.; Novoselov, K. S. Nat. Mater. 2007, 6, 183. (5) Novoselov, K. S.; Geim, A. K.; Morozov, S. V.; Jiang, D.; Katsnelson, M. I.; Grigorieva, I. V.; Dubonos, S. V.; Firsov, A. A. Nature 2005, 438, 197. (6) Tomonaga, S. Prog. Theor. Phys. 1950, 5, 544. (7) Luttinger, J. M. J. Math. Phys. 1963, 4, 1154. (8) Yanson, A. I.; Bollinger, G. R.; van den Brom, H. E.; Agrait, N.; van Ruitenbeek, J. M. Nature 1998, 395, 783. (9) Oncel, N.; van Houselt, A.; Huijben, J.; Hallba¨ck, A.-S.; Gurlu, O.; Zandvliet, H. J. W.; Poelsema, B. Phys. ReV. Lett. 2005, 95, 116801. (10) van Houselt, A.; Oncel, N.; Poelsema, B.; Zandvliet, H. J. W. Nano Lett. 2006, 6, 1439–1442. (11) Gambardella, P.; Dallmeyer, A.; Maiti, K.; Malagoli, M. C.; Eberhardt, W.; Kern, K.; Carbone, C. Nature 2002, 416, 301. (12) Nilius, N.; Wallis, T. M.; Ho, W. Science 2002, 297, 1853. (13) Yeom, H. W.; Takeda, S.; Rotenberg, E.; Matsuda, I.; Horikoshi, K.; Schaefer, J.; Lee, C. M.; Kevan, S. D.; Ohta, T.; Nagao, T.; Hasegawa, S. Phys. ReV. Lett. 1999, 82, 4898. (14) Losio, R.; Altmann, K. N.; Kirakosian, A.; Lin, J.-L.; Petrovykh, D. Y.; Himpsel, F. J. Phys. ReV. Lett. 2001, 86, 4632. (15) Segovia, P.; Purdie, D.; Hengsberger, M.; Baer, Y. Nature 1999, 402, 504. (16) Gurlu, O.; Adam, O. A. O.; Zandvliet, H. J. W.; Poelsema, B. Appl. Phys. Lett. 2003, 83, 4610. (17) Wang, J.; Li, M.; Altman, E. I. Phys. ReV. B 2004, 70, 233312. (18) Wang, J.; Li, M.; Altman, E. I. Surf. Sci. 2005, 596, 126. (19) Scha¨fer, J.; Blumenstein, C.; Meyer, S.; Wisniewski, M.; Claesen, R. Phys. ReV. Lett. 2008, 101, 236802. (20) van Houselt, A.; Fischer, M.; Poelsema, B.; Zandvliet, H. J. W. Phys. ReV. B 2008, 78, 233410. (21) Zandvliet, H. J. W.; Swartzentruber, B. S.; Wulfhekel, W.; Hattink, B.-J.; Poelsema, B. Phys. ReV. B 1998, 57, R6803. (22) Zandvliet, H. J. W. Phys. Rep. 2003, 388, 1. (23) van Houselt, A.; van Gastel, R.; Poelsema, B.; Zandvliet, H. J. W. Phys. ReV. Lett. 2006, 97, 266104. (24) Fischer, M.; van Houselt, A.; Kockmann, D.; Poelsema, B.; Zandvliet, H. J. W. Phys. ReV. B 2007, 76, 245429. (25) Gurlu, O.; Zandvliet, H. J. W.; Poelsema, B. Phys. ReV. Lett. 2004, 93, 066101. (26) Nakatsuji, K.; Niikura, R.; Shibata, Y.; Yamada, M.; Iimori, T.; Komori, F. Phys. ReV. B 2009, 80, 081406(R).
(1) Klitzing, K. v.; Dorda, G.; Pepper, M. Phys. ReV. Lett. 1980, 45, 494.
Conclusions In conclusion, using STM and STS we have studied the structural and electronic properties of Au induced nanowires on Ge(001) prepared by two different methods. In both cases the Au induced nanowires are comprised of Ge dimers that have their bond aligned in a direction perpendicular to the nanowire direction and have a height of at least four atomic layers. The buckling of the Ge dimers leads to a 2× periodicity along the nanowires direction. At antiphase boundaries in this buckling registry Ge dimers are found which flip back and forth between their two buckled configurations. The differential conductivities of the nanowires and the regions in between the nanowires have very comparable values and are only marginally metallic. Note Added in Proof. After the acceptance of our article we became aware of an article by Nakatsuji et al.26 In this article the electronic properties of the Au/Ge(001) system are investigated by angle-resolved photoelectron spectroscopy. The experimental findings in this paper regarding the structural and electronic properties of the Au/Ge(001) system are in good agreement with our observations.